Presentation on theme: "Chapter 16 1 Powder Metallurgy Chapter 16 Manufacturing Processes, MET1311 Dr Simin Nasseri Southern Polytechnic State University."— Presentation transcript:
Chapter 16 1 Powder Metallurgy Chapter 16 Manufacturing Processes, MET1311 Dr Simin Nasseri Southern Polytechnic State University
Manufacturing Processes Prof Simin Nasseri Chapter 16 2 POWDER METALLURGY 1.The Characterization of Engineering Powders 2.Production of Metallic Powders 3.Conventional Pressing and Sintering 4.Alternative Pressing and Sintering Techniques 5.Materials and Products for PM 6.Design Considerations in Powder Metallurgy
Manufacturing Processes Prof Simin Nasseri Chapter 16 3 Modern powder metallurgy dates only back to the early 1800 Powder Metallurgy (PM) Metal processing technology in which parts are produced from metallic powders PM parts can be mass produced to net shape or near net shape, eliminating or reducing the need for subsequent machining Certain metals that are difficult to fabricate by other methods can be shaped by PM Tungsten filaments for lamp bulbs are made by PM PM process wastes very little material - ~ 97% of starting powders are converted to product PM parts can be made with a specified level of porosity, to produce porous metal parts Examples: filters, oil impregnated bearings and gears
Manufacturing Processes Prof Simin Nasseri Chapter 16 4 Limitations and Disadvantages High tooling and equipment costs Metallic powders are expensive Problems in storing and handling metal powders Degradation over time, fire hazards with certain metals Limitations on part geometry because metal powders do not readily flow laterally in the die during pressing Variations in density throughout part may be a problem, especially for complex geometries
Manufacturing Processes Prof Simin Nasseri Chapter 16 5 Usual PM production sequence Blending and mixing (Rotating drums, blade and screw mixers) Pressing - powders are compressed into desired shape to produce green compact Accomplished in press using punch-and-die tooling designed for the part Sintering – green compacts are heated to bond the particles into a hard, rigid mass Performed at temperatures below the melting point of the metal
Manufacturing Processes Prof Simin Nasseri Chapter 16 6 PM Work Materials Largest tonnage of metals are alloys of iron, steel, and aluminum Other PM metals include copper, nickel, and refractory metals such as molybdenum and tungsten Metallic carbides such as tungsten carbide are often included within the scope of powder metallurgy
Manufacturing Processes Prof Simin Nasseri Chapter 16 7 A collection of powder metallurgy parts. PM Parts
Manufacturing Processes Prof Simin Nasseri Chapter 16 8 Engineering Powders A powder can be defined as a finely divided particulate solid Engineering powders include metals and ceramics Geometric features of engineering powders: Particle size and distribution Particle shape and internal structure Surface area
Manufacturing Processes Prof Simin Nasseri Chapter 16 9 Measuring Particle Size Most common method uses screens of different mesh sizes Mesh count - refers to the number of openings per linear inch of screen A mesh count of 200 means there are 200 openings per linear inch Higher mesh count = smaller particle size Figure 16.2 Screen mesh for sorting particle sizes.
Manufacturing Processes Prof Simin Nasseri Chapter Figure 16.3 Several of the possible (ideal) particle shapes in powder metallurgy. Particle Shapes in PM
Manufacturing Processes Prof Simin Nasseri Chapter Interparticle Friction and Powder Flow Friction between particles affects ability of a powder to flow readily and pack tightly A common test of interparticle friction is the angle of repose, which is the angle formed by a pile of powders as they are poured from a narrow funnel. Figure 16.4 Interparticle friction as indicated by the angle of repose of a pile of powders poured from a narrow funnel. Larger angles indicate greater interparticle friction.
Manufacturing Processes Prof Simin Nasseri Chapter Lets check! Smaller particle sizes show steeper angles or larger particle sizes?! Smaller particle sizes generally show greater friction and steeper angles! Finer particles
Manufacturing Processes Prof Simin Nasseri Chapter Lets check! Which shape has the lowest interpartical friction? Spherical shapes have the lowest interpartical friction! Little friction between spherical particles! As shape deviates from spherical, friction between particles tends to increase
Manufacturing Processes Prof Simin Nasseri Chapter Observations Easier flow of particles correlates with lower interparticle friction Lubricants are often added to powders to reduce interparticle friction and facilitate flow during pressing
Manufacturing Processes Prof Simin Nasseri Chapter Particle Density Measures True density - density of the true volume of the material The density of the material if the powders were melted into a solid mass Bulk density - density of the powders in the loose state after pouring Which one is smaller?! Because of pores between particles, bulk density is less than true density
Manufacturing Processes Prof Simin Nasseri Chapter Packing Factor Typical values for loose powders range between 0.5 and 0.7 Bulk density true density Packing factor = If powders of various sizes are present, smaller powders will fit into spaces between larger ones, thus higher packing factor Packing can be increased by vibrating the powders, causing them to settle more tightly Pressure applied during compaction greatly increases packing of powders through rearrangement and deformation of particles How can we increase the bulk density?
Manufacturing Processes Prof Simin Nasseri Chapter Porosity Ratio of volume of the pores (empty spaces) in the powder to the bulk volume In principle Porosity + Packing factor = 1.0 The issue is complicated by possible existence of closed pores in some of the particles If internal pore volumes are included in above porosity, then equation is exact
Manufacturing Processes Prof Simin Nasseri Chapter Chemistry and Surface Films Metallic powders are classified as either Elemental - consisting of a pure metal (slide 39) Pre-alloyed - each particle is an alloy Possible surface films include oxides, silica, adsorbed organic materials, and moisture As a general rule, these films must be removed prior to shape processing
Chapter Production of Metallic Powders
Manufacturing Processes Prof Simin Nasseri Chapter Production of Metallic Powders In general, producers of metallic powders are not the same companies as those that make PM parts Any metal can be made into powder form Three principal methods by which metallic powders are commercially produced 1.Atomization (by gas, water, also centrifugal one) 2.Chemical 3.Electrolytic In addition, mechanical methods are occasionally used to reduce powder sizes
Manufacturing Processes Prof Simin Nasseri Chapter High velocity gas stream flows through expansion nozzle, siphoning molten metal from below and spraying it into container Figure 16.5 (a) gas atomization method Check other figures as well (page 344) Gas Atomization Method
Manufacturing Processes Prof Simin Nasseri Chapter Figure 16.6 Iron powders produced by decomposition of iron pentacarbonyl (photo courtesy of GAF Chemical Corp); particle sizes range from about microns (10 to 125 -in). Iron Powders for PM
Manufacturing Processes Prof Simin Nasseri Chapter Conventional Press and Sinter After metallic powders have been produced, the conventional PM sequence consists of: 1.Blending and mixing of powders 2.Compaction - pressing into desired shape 3.Sintering - heating to temperature below melting point to cause solid state bonding of particles and strengthening of part In addition, secondary operations are sometimes performed to improve dimensional accuracy, increase density, and for other reasons
Manufacturing Processes Prof Simin Nasseri Chapter Figure 16.7 Conventional powder metallurgy production sequence: (1) blending, (2) compacting, and (3) sintering; (a) shows the condition of the particles while (b) shows the operation and/or workpart during the sequence.
Manufacturing Processes Prof Simin Nasseri Chapter Blending and Mixing of Powders For successful results in compaction and sintering, the starting powders must be homogenized (powders should be blended and mixed) Blending - powders of same chemistry but possibly different particle sizes are intermingled Different particle sizes are often blended to reduce porosity Mixing - powders of different chemistries are combined
Manufacturing Processes Prof Simin Nasseri Chapter Compaction Application of high pressure to the powders to form them into the required shape Conventional compaction method is pressing, in which opposing punches squeeze the powders contained in a die The workpart after pressing is called a green compact, the word green meaning not yet fully processed The green strength of the part when pressed is adequate for handling but far less than after sintering
Manufacturing Processes Prof Simin Nasseri Chapter Conventional Pressing in PM Figure 16.9 Pressing in PM: (1) filling die cavity with powder by automatic feeder; (2) initial and (3) final positions of upper and lower punches during pressing, (4) part ejection. Watch the single- and double-punch operations Fill Press Eject
Manufacturing Processes Prof Simin Nasseri Chapter Sintering Heat treatment to bond the metallic particles, thereby increasing strength and hardness Usually carried out at between 70% and 90% of the metal's melting point (absolute scale) Generally agreed among researchers that the primary driving force for sintering is reduction of surface energy Part shrinkage occurs during sintering due to pore size reduction
Manufacturing Processes Prof Simin Nasseri Chapter Figure Sintering on a microscopic scale: (1) particle bonding is initiated at contact points; (2) contact points grow into "necks"; (3) the pores between particles are reduced in size; and (4) grain boundaries develop between particles in place of the necked regions. Sintering Sequence Watch the sintering operation
Manufacturing Processes Prof Simin Nasseri Chapter Figure (a) Typical heat treatment cycle in sintering; and (b) schematic cross section of a continuous sintering furnace. Sintering Cycle and Furnace
Manufacturing Processes Prof Simin Nasseri Chapter Densification and Sizing Secondary operations are performed to increase density, improve accuracy, or accomplish additional shaping of the sintered part Repressing - pressing sintered part in a closed die to increase density and improve properties Sizing - pressing a sintered part to improve dimensional accuracy Coining - pressworking operation on a sintered part to press details into its surface Machining - creates geometric features that cannot be achieved by pressing, such as threads, side holes, and other details
Manufacturing Processes Prof Simin Nasseri Chapter Impregnation and Infiltration Porosity is a unique and inherent characteristic of PM technology It can be exploited to create special products by filling the available pore space with oils, polymers, or metals Two categories: 1.Impregnation 2.Infiltration
Manufacturing Processes Prof Simin Nasseri Chapter Impregnation The term used when oil or other fluid is permeated into the pores of a sintered PM part Common products are oil impregnated bearings, gears, and similar components Alternative application is when parts are impregnated with polymer resins that seep into the pore spaces in liquid form and then solidify to create a pressure tight part
Manufacturing Processes Prof Simin Nasseri Chapter Infiltration Operation in which the pores of the PM part are filled with a molten metal The melting point of the filler metal must be below that of the PM part Involves heating the filler metal in contact with the sintered component so capillary action draws the filler into the pores Resulting structure is relatively nonporous, and the infiltrated part has a more uniform density, as well as improved toughness and strength T M (filler)
Manufacturing Processes Prof Simin Nasseri Chapter Alternatives to Pressing and Sintering Conventional press and sinter sequence is the most widely used shaping technology in powder metallurgy Additional methods for processing PM parts include: Isostatic pressing Powder injection molding Powder rolling, extrusion and forging Combined pressing and sintering Liquid phase sintering
Manufacturing Processes Prof Simin Nasseri Chapter Powder Injection Molding Metal injection molding Pellets made of powders and binder Heated to molding temperature and injected into a mold Can create complex designs
Manufacturing Processes Prof Simin Nasseri Chapter Materials and Products for PM Raw materials for PM are more expensive than for other metalworking because of the additional energy required to reduce the metal to powder form Accordingly, PM is competitive only in a certain range of applications What are the materials and products that seem most suited to powder metallurgy?
Manufacturing Processes Prof Simin Nasseri Chapter PM Materials – Elemental Powders A pure metal in particulate form Applications where high purity is important Common elemental powders: Iron Aluminum Copper Elemental powders can be mixed with other metal powders to produce alloys that are difficult to formulate by conventional methods Example: tool steels
Manufacturing Processes Prof Simin Nasseri Chapter PM Materials – Pre-Alloyed Powders Each particle is an alloy comprised of the desired chemical composition Common pre-alloyed powders: Stainless steels Certain copper alloys High speed steel
Manufacturing Processes Prof Simin Nasseri Chapter PM Products Gears, bearings, sprockets, fasteners, electrical contacts, cutting tools, and various machinery parts Advantage of PM: parts can be made to near net shape or net shape When produced in large quantities, gears and bearings are ideal for PM because: The geometry is defined in two dimensions (cross section is uniform) There is a need for porosity in the part to serve as a reservoir for lubricant